LMucko/crystallography-open-database huggingface dataset:
X-ray single-crystal study of spinels: in situ heating Sample: NAT, Heating, 4th run, T = 600 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007086
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: NAT, Heating, 4th run, T = 600 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al1.937 Cr0.061 Fe0.002 Mg0.996 O4 Zn0.004'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1362
_cell_length_b                   8.1362
_cell_length_c                   8.1362
_cell_formula_units_Z            8
_cell_volume                     538.598
_database_code_amcsd             0008671
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    3.552
_exptl_crystal_thermal_history   'heating, 4th run, T = 600 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.937 Mg.996 Zn.004 Cr.061 Fe.002 O4'
_cod_database_code               9007086
X-ray single-crystal study of spinels: in situ heating Sample: NAT, Heating, 4th run, T = 700 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007087
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: NAT, Heating, 4th run, T = 700 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al1.937 Cr0.061 Fe0.002 Mg0.996 O4 Zn0.004'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1441
_cell_length_b                   8.1441
_cell_length_c                   8.1441
_cell_formula_units_Z            8
_cell_volume                     540.169
_database_code_amcsd             0008672
_diffrn_ambient_temperature      973.15
_exptl_crystal_density_diffrn    3.542
_exptl_crystal_thermal_history   'heating, 4th run, T = 700 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.937 Mg.996 Zn.004 Cr.061 Fe.002 O4'
_cod_database_code               9007087
X-ray single-crystal study of spinels: in situ heating Sample: NAT, Heating, 4th run, T = 800 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007088
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: NAT, Heating, 4th run, T = 800 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al1.937 Cr0.061 Fe0.002 Mg0.996 O4 Zn0.004'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1516
_cell_length_b                   8.1516
_cell_length_c                   8.1516
_cell_formula_units_Z            8
_cell_volume                     541.662
_database_code_amcsd             0008673
_diffrn_ambient_temperature      1073.15
_exptl_crystal_density_diffrn    3.532
_exptl_crystal_thermal_history   'heating, 4th run, T = 800 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.937 Mg.996 Zn.004 Cr.061 Fe.002 O4'
_cod_database_code               9007088
X-ray single-crystal study of spinels: in situ heating Sample: NAT, Heating, 4th run, T = 900 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007089
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: NAT, Heating, 4th run, T = 900 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al1.937 Cr0.061 Fe0.002 Mg0.996 O4 Zn0.004'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1592
_cell_length_b                   8.1592
_cell_length_c                   8.1592
_cell_formula_units_Z            8
_cell_volume                     543.179
_database_code_amcsd             0008674
_diffrn_ambient_temperature      1173.15
_exptl_crystal_density_diffrn    3.522
_exptl_crystal_thermal_history   'heating, 4th run, T = 900 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.937 Mg.996 Zn.004 Cr.061 Fe.002 O4'
_cod_database_code               9007089
X-ray single-crystal study of spinels: in situ heating Sample: NAT, Cooling, T = 800 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007090
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: NAT, Cooling, T = 800 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al1.937 Cr0.061 Fe0.002 Mg0.996 O4 Zn0.004'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1510
_cell_length_b                   8.1510
_cell_length_c                   8.1510
_cell_formula_units_Z            8
_cell_volume                     541.543
_database_code_amcsd             0008675
_diffrn_ambient_temperature      1073.15
_exptl_crystal_density_diffrn    3.533
_exptl_crystal_thermal_history   'heating Sample: NAT, Cooling, T = 800 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.937 Mg.996 Zn.004 Cr.061 Fe.002 O4'
_cod_database_code               9007090
X-ray single-crystal study of spinels: in situ heating Sample: NAT, Cooling, T = 800 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007091
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: NAT, Cooling, T = 800 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al1.937 Cr0.061 Fe0.002 Mg0.996 O4 Zn0.004'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1510
_cell_length_b                   8.1510
_cell_length_c                   8.1510
_cell_formula_units_Z            8
_cell_volume                     541.543
_database_code_amcsd             0008676
_diffrn_ambient_temperature      1073.15
_exptl_crystal_density_diffrn    3.533
_exptl_crystal_thermal_history   'heating Sample: NAT, Cooling, T = 800 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.937 Mg.996 Zn.004 Cr.061 Fe.002 O4'
_cod_database_code               9007091
_cod_duplicate_entry 9007090
X-ray single-crystal study of spinels: in situ heating Sample: NAT, Cooling, T = 700 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007092
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: NAT, Cooling, T = 700 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al1.937 Cr0.061 Fe0.002 Mg0.996 O4 Zn0.004'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1431
_cell_length_b                   8.1431
_cell_length_c                   8.1431
_cell_formula_units_Z            8
_cell_volume                     539.970
_database_code_amcsd             0008677
_diffrn_ambient_temperature      973.15
_exptl_crystal_density_diffrn    3.543
_exptl_crystal_thermal_history   'heating Sample: NAT, Cooling, T = 700 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.937 Mg.996 Zn.004 Cr.061 Fe.002 O4'
_cod_database_code               9007092
X-ray single-crystal study of spinels: in situ heating Sample: NAT, Cooling, T = 600 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007093
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: NAT, Cooling, T = 600 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al1.937 Cr0.061 Fe0.002 Mg0.996 O4 Zn0.004'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1350
_cell_length_b                   8.1350
_cell_length_c                   8.1350
_cell_formula_units_Z            8
_cell_volume                     538.360
_database_code_amcsd             0008678
_diffrn_ambient_temperature      873.15
_exptl_crystal_density_diffrn    3.554
_exptl_crystal_thermal_history   'heating Sample: NAT, Cooling, T = 600 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.937 Mg.996 Zn.004 Cr.061 Fe.002 O4'
_cod_database_code               9007093
X-ray single-crystal study of spinels: in situ heating Sample: NAT, Cooling, T = 500 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007094
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: NAT, Cooling, T = 500 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al1.937 Cr0.061 Fe0.002 Mg0.996 O4 Zn0.004'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1271
_cell_length_b                   8.1271
_cell_length_c                   8.1271
_cell_formula_units_Z            8
_cell_volume                     536.793
_database_code_amcsd             0008679
_diffrn_ambient_temperature      773.15
_exptl_crystal_density_diffrn    3.564
_exptl_crystal_thermal_history   'heating Sample: NAT, Cooling, T = 500 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.937 Mg.996 Zn.004 Cr.061 Fe.002 O4'
_cod_database_code               9007094
X-ray single-crystal study of spinels: in situ heating Sample: NAT, Cooling, T = 400 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007095
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: NAT, Cooling, T = 400 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al1.937 Cr0.061 Fe0.002 Mg0.996 O4 Zn0.004'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1183
_cell_length_b                   8.1183
_cell_length_c                   8.1183
_cell_formula_units_Z            8
_cell_volume                     535.051
_database_code_amcsd             0008680
_diffrn_ambient_temperature      673.15
_exptl_crystal_density_diffrn    3.576
_exptl_crystal_thermal_history   'heating Sample: NAT, Cooling, T = 400 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.937 Mg.996 Zn.004 Cr.061 Fe.002 O4'
_cod_database_code               9007095
X-ray single-crystal study of spinels: in situ heating Sample: NAT, Cooling, T = 200 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007096
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: NAT, Cooling, T = 200 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al1.937 Cr0.061 Fe0.002 Mg0.996 O4 Zn0.004'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1036
_cell_length_b                   8.1036
_cell_length_c                   8.1036
_cell_formula_units_Z            8
_cell_volume                     532.150
_database_code_amcsd             0008681
_diffrn_ambient_temperature      473.15
_exptl_crystal_density_diffrn    3.595
_exptl_crystal_thermal_history   'heating Sample: NAT, Cooling, T = 200 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.937 Mg.996 Zn.004 Cr.061 Fe.002 O4'
_cod_database_code               9007096
X-ray single-crystal study of spinels: in situ heating Sample: NAT, Cooling, T = 25 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007097
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: NAT, Cooling, T = 25 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al1.937 Cr0.061 Fe0.002 Mg0.996 O4 Zn0.004'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.0926
_cell_length_b                   8.0926
_cell_length_c                   8.0926
_cell_formula_units_Z            8
_cell_volume                     529.986
_database_code_amcsd             0008682
_diffrn_ambient_temperature      298.15
_exptl_crystal_density_diffrn    3.610
_exptl_crystal_thermal_history   'heating Sample: NAT, Cooling, T = 25 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.937 Mg.996 Zn.004 Cr.061 Fe.002 O4'
_cod_database_code               9007097
X-ray single-crystal study of spinels: in situ heating Sample: TRANS, Heating, 1st run, T = 850 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007098
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: TRANS, Heating, 1st run, T = 850 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al1.937 Cr0.061 Fe0.002 Mg0.996 O4 Zn0.004'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1525
_cell_length_b                   8.1525
_cell_length_c                   8.1525
_cell_formula_units_Z            8
_cell_volume                     541.842
_database_code_amcsd             0008683
_diffrn_ambient_temperature      1123.15
_exptl_crystal_density_diffrn    3.531
_exptl_crystal_thermal_history   'heating, 1st run, T = 850 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.937 Mg.996 Zn.004 Cr.061 Fe.002 O4'
_cod_database_code               9007098
X-ray single-crystal study of spinels: in situ heating Sample: TRANS, Heating, 1st run, T = 25 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007099
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: TRANS, Heating, 1st run, T = 25 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al1.937 Cr0.061 Fe0.002 Mg0.996 O4 Zn0.004'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.0924
_cell_length_b                   8.0924
_cell_length_c                   8.0924
_cell_formula_units_Z            8
_cell_volume                     529.946
_database_code_amcsd             0008684
_diffrn_ambient_temperature      298.15
_exptl_crystal_density_diffrn    3.610
_exptl_crystal_thermal_history   'heating, 1st run, T = 25 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.937 Mg.996 Zn.004 Cr.061 Fe.002 O4'
_cod_database_code               9007099
X-ray single-crystal study of spinels: in situ heating Sample: TRANS, Heating, 1st run, T = 200 C
Carbonin, S.; Martignago, F.; Menegazzo, G.; Dal Negro, A.; Physics and Chemistry of Minerals 29 (2002) 503–514; doi:10.1007/s00269-002-0262-6

data_9007100
_publ_section_title
;
 X-ray single-crystal study of spinels: in situ heating
 Sample: TRANS, Heating, 1st run, T = 200 C
;
_journal_name_full               'Physics and Chemistry of Minerals'
_journal_page_first              503
_journal_page_last               514
_journal_paper_doi               10.1007/s00269-002-0262-6
_journal_volume                  29
_journal_year                    2002
_chemical_formula_sum            'Al1.937 Cr0.061 Fe0.002 Mg0.996 O4 Zn0.004'
_chemical_name_mineral           Spinel
_space_group_IT_number           227
_symmetry_space_group_name_Hall  '-F 4vw 2vw 3'
_symmetry_space_group_name_H-M   'F d -3 m :2'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                90
_cell_length_a                   8.1025
_cell_length_b                   8.1025
_cell_length_c                   8.1025
_cell_formula_units_Z            8
_cell_volume                     531.933
_database_code_amcsd             0008685
_diffrn_ambient_temperature      473.15
_exptl_crystal_density_diffrn    3.597
_exptl_crystal_thermal_history   'heating, 1st run, T = 200 C'
_cod_original_sg_symbol_H-M      'F d 3 m'
_cod_original_formula_sum        'Al1.937 Mg.996 Zn.004 Cr.061 Fe.002 O4'
_cod_database_code               9007100